Upload
phungtu
View
252
Download
3
Embed Size (px)
Citation preview
BUCKLING ANALYSIS OF LAMINATED
COMPOSITE PLATES
A Thesis Submitted in Partial Fulfilment of the Requirements for the
degree of
Bachelor of Technology
In
Mechanical Engineering
Praseed Sahu
ROLL NO: 110ME0327
(Department Of Mechanical Engineering)
Department Of Mechanical Engineering
National Institute Of Technology Rourkela
Rourkela-769008
BUCKLING ANALYSIS OF LAMINATED
COMPOSITE PLATES
A Thesis Submitted in Partial Fulfilment of the Requirements for the
degree of
Bachelor of Technology
In
Mechanical Engineering
Praseed Sahu
ROLL NO: 110ME0327
(Department Of Mechanical Engineering)
Under the guidance of
Prof. Subrata Kumar Panda
Department Of Mechanical Engineering
National Institute Of Technology Rourkela
Rourkela-769008
NATIONAL INSTITUTE OF TECHNOLOGY
ROURKELA – 769008, ODISHA
INDIA
CERTIFICATE
This is to certify that the thesis entitled, “BUCKLING ANALYSIS OF LAMINATED
COMPOSITE PLATES” submitted by Mr Praseed Sahu in partial fulfilment of the requirement for the
award of Bachelor of Technology Degree in Mechanical Engineering with specialization in
Mechanical Engineering at the National Institute of Technology, Rourkela (Deemed University) is an
authentic work carried out by him under my supervision and guidance.
To the best of my knowledge, the matter embodied in the thesis has not been submitted to any other
University/ Institute for the award of any degree or diploma.
Dr. S.K. Panda
Department Of Mechanical Engineering
NIT Rourkela
Acknowledgments
I would like to express my gratitude to my guide, Dr. S K Panda for his encouragement, advice,
mentoring and research support throughout my studies. His technical and editorial advice was essential for
the completion of this dissertation. His ability to teach, depth of knowledge and ability to achieve perfection
will always be my inspiration.
My sincere thanks to Dr. S. K. Dutta, Professor Department of Mechanical Engineering, National
Institute of Technology Rourkela, for providing necessary facility for my work.
I am very thankful to Mr Arabinda Khuntia and Mr Tanmay Kumar Sahu of Mechanical
engineering department who assisted me developing the test rig. I would also like to thank Mr Vishesh Kar
and Mr Vijay Kumar Singh of Department of Mechanical Engineering.
I appreciate the kind gesture shown by Mr Swayam Bikash Mishra in helping me develop the
necessary parts for the project.
This project would also not have been completed had Sandeep Mishra, Prakash Sarangi, Sourava
Jyoti Nayak not been there for helping me in making this dream come true.
I am highly grateful to TEQIP II for providing the necessary financial assistance required in making
this project a reality.
Praseed Sahu
Department of Mechanical Engineering
NIT Rourkela
ABSTRACT
Laminated composites have been used in many engineering structures from early time the
recent advancements in material technology has led to the creation of a new composite with
enhanced properties. Composite materials are generally used in many fields of engineering like
buildings, bridges, boat hulls, swimming pool panels, race car bodies, shower stalls, bathtubs
and storage tanks. In addition to that industries where weight reduction is of prime concern
(aviation and spacecraft etc.). Composites are capable enough to take different types of loading
both tensile and compressive based on the requirement. It is well known that the structural
elements under compressive loads and/or due to thin built up they may be prone to buckle. In
order to evaluate the buckling strength of laminated structures many studies has already been
completed numerically and experimentally. A lab scale buckling test rig has been developed to
obtain the critical load. In addition to that a simulation study has been done in ANSYS using
ANSYS parametric design language. Some new results have been obtained for different
parameter and discussed in detail.
Keywords: Buckling, Laminated composites, Experimental analysis, FEM, ANSYS
CONTENTS
Chapter 1…………………………………………………………………01-04
Introduction and literature review
Chapter 2…………………………………………………………………05-12
Theoretical formulation and modelling
Chapter 3…………………………………………………………………13-18
Experimental study
Chapter 4…………………………………………………………………19-22
Results and discussions
Chapter 5…………………………………………………………………23-24
Conclusion
Chapter 6……………………………………………………………..…..25-27
References
List of figures:
Serial No Figure Page
1 Definition of plate axes 6
2 Layers of a laminate composite plate 8
3 Forces on laminate plate 9
4 Moments on laminate plate 9
5 Laminated composite plate with detailed layer number 10
6 Hand layup technique 15
7(a) - 7(b) Glass fibre and epoxy 16
8(a) – 8(f) Preparation of composite plates 17-18
9 Buckling test rig 18
List of Tables:
Serial No Table Page
1 Buckling load comparison of [0/90/0] laminate 22
2 Buckling load comparison of [0/90/90/0] laminate 22
3 Effect of thickness ratio (a/h) on buckling load 23
4 Effect of thickness orthotropicity on buckling load
23
1
CHAPTER 1
INTRODUCTION AND
LITERATURE REVIEW
2
INTRODUCTION
There are many types of failures in engineering structures. Some of them include creep, fatigue,
alternate stresses, bending, buckling etc. Buckling takes place in columns, plates, shells, and
other structures of regular or irregular geometry. In this project only buckling of laminated
composite plates has been considered. If the loads applied to a flat plate are low then there is
low no observed distortion of the plate however as the load is increased then the equilibrium
configuration of the plate changes into no flat configuration. Thus the plate in the case becomes
unstable. The minimum load at which the equilibrium is disturbed is called as the critical
buckling load.
A composite has dual character. It is made up of two or more materials which when combined
give different properties than their original characteristics. These materials have important
properties like they are light in weight because the combined properties give rise to significant
weight loss character. Thus they have high strength and high stiffness compared to their weight.
Also in a composite the properties are affected by the degree of composition of the parent
materials. Thus the properties can be altered by changing the composition of the composite.
In composites the two components are called as fibre and matrix. The fibres are the main load
bearing members and the matrix, which has low modulus and high elongation, provides the
necessary flexibility and also keeps the fibres in position and protect them from the
environment.
As discussed in the previous paragraph, flexibility is one of the major advantage of composite
which in turn creates the necessity and requirement of the analysis of the structure. The
properties of such materials depend on the constituent materials, their distribution in the matrix
and their orientation in the composite. Thus a new material with unusual combination can be
obtained with properties that are dissimilar to the parent constituents.
Some of the uses of laminated composite plates are in critical areas of infrastructure like
aviation, waterways, military, structures etc. In most of these cases the fibre reinforced
composites are not in the form of columns but thin flat plates which carry axial compressive
loads. During their operating period the compressive loads may exceed a safety value and this
may cause buckling of the composite plates which can cause catastrophic failures. Many
theoretical computations are there which formulate the behaviour of such composites under
3
loads and solving them gives the critical buckling load. But such computations tend to be
cumbersome and lengthy. To avoid these technicalities experimental methods are much
preferred. This study aims to develop an indigenous setup which can estimate the critical
buckling load.
LITERATURE REVIEW
In 1964 Schlack [3] analysed the buckling behaviour of a simple supported square plate with a
circular hole was analysed by applying Rayleigh- Ritz method. Martin [4] in 1972 presented
the buckling of square composite plates having a cut out that are subjected to uniaxial
compression. In 1986 results for buckling of orthotropic rectangular plates with longitudinally
eccentric circular cut-out was presented by Marshall, Little, El-Tayeby, and Williams [5]. In
1987 Nemeth, Stein, and Johnson [6] analysed the buckling behaviour of square orthotropic
graphite – epoxy plates that have a central circular cut-out and gave additional analytical
results. In 1989 Lee [7] used the finite element method (FEM) to examine the buckling
behaviour of square plate with a central circular hole. A buckling behaviour of sequence
laminated composite plate, each with a central circular cut-out was presented by Lin and Kuok
[8] in 1989. The mechanical and thermal buckling behaviour of rectangular steel plates with
central circular and square cutout was studied by William [9]. In 1990 Rouse [10] presented an
experimental investigation of the buckling and post buckling behavior of square graphite-
epoxy and graphite – thermoplastic plates loaded in shear. In 1991 Yaqui [11] described the
study of buckling behaviour of laminated composite plates with a central cutout that has been
obtained by using the finite element method. In 2004 [12] Jameel studied the buckling behavior
of an elastic plate with circular hole.
From the above literatures, it can be seen that many studies has been reported on buckling
analysis of laminated composites numerically and experimentally as well. It is also observed
that some of the studies have been done with the help of commercial finite element (FE) tool
like ANSYS, ABAQUS and NASTRAN etc. It is understood that the numerical study using
commercial FE tool not only easy to model but also less time expensive. Hence, the objective
of the present work has been stated in following paragraph based on the above observation.
4
AIM AND SCOPE OF PRESENT WORK
As discussed earlier, the thin laminated composite plates are capable to carry extra amount of
load under compressive loading. It is well known that the structures under compressive loading
may lose their stability and a geometric instability induced in the structure which in turn say,
buckling of the structure.
To achieve the same majority of work has been carried out in modelling and numerical
investigation of the buckling behaviour of the laminated composite plates time to time. It is
also true that the experimental methods however are not too easy to implement. It is because
of the fact that fabrication of composite plate by maintaining the required properties for which
they have been the quest of design engineers as well as available INSTRON machine which
are very costly. Hence, the present project aims at develop an lab scale buckling test rig using
hydraulic pressure to calculate the critical buckling load of various laminated plate. It is worthy
to mention that the required specimens have been prepared using hand lay-up technique.
Finally, the results are also obtained numerically using commercial finite element software.
5
CHAPTER 2
THEORETICAL FORMULATION AND
MODELLING
6
THEORETICAL FORMULATION
The buckling phenomenon of a plate includes two boundary conditions on each edge of a plate.
The buckling characteristic of a plate and a column is very different. In case of a column the
critical buckling load is the failure load i.e. the column fails at the buckling load but in case of
a plate the failure load is around 10-15 times that of the critical buckling load. In some cases
failure does not occur in the plates even at these loads.
THEORY OF BENDING OF THIN PLATES
Bending of thin plates is in many ways similar to the bending of beams. In pure bending of
beams, "the stress distribution is obtained by assuming that cross-sections of the plate remains
plane during bending and only rotate w.r.t. their neutral axes so that it is always normal to the
deflection curve."
Figure 1
Axis definition of a laminate composite plate [2]
7
The assumptions in elastic bending are:
The plate material is linear and follows the Hooke’s law.
The plate is completely flat and is of uniform thickness throughout the cross section.
The thickness of the plate is small compared to the length and breadth of the plate.
Therefore normal stress in transverse direction can be neglected compared to normal
stress in plane of plate.
The deflection that the plate undergoes is very small, generally around half of the
thickness.
The stress in the mid plane of the plate is zero and it behaves as the neutral plane.
The application of load is normal to the centre plane of the plate.
The applied load is resisted by the bending and twisting of the plate. The shearing
effects are neglected.
Like bending in a beam the stresses and strains are proportional to their distances from
the neutral surfaces.
Composite materials
Composites are materials which are prepared by the combination of two or more materials and
the properties of the composites are markedly different from the properties of the parent
materials. Composite laminates are sum total of layers of fibres which can be assembled to
give required material properties which includes in-plane stiffness, bending stiffness, strength,
and coefficient of thermal expansion. In laminated composite plates the orientation of the
matrix is very important as it gives different properties.
Each layer of the fibre reinforced composite plate is called as a lamina. Lamina is a macro
component of a laminate and its properties are dependent on the stacking sequence and the
hardener used. Its properties are derived experimentally. Structural elements such as beams,
bars and plates are generated by assembling the layers to achieve desired strength and
stiffness. The orientation of the fibres and the stacking sequence give the laminate the desired
strength and stiffness.
8
Governing Equations
A laminate is produced by using laminas which are stacked in sequences to obtain the laminate.
The properties of the laminate like its stiffness is obtained by knowing the properties of the
constituent materials. To know this the orientation of the principal matrix element must be
known. Therefore we must know the directions of stress and strain through the lamina.
To study the behaviour of the laminates we assume the following:
The bonds in the laminate are strong and perfect.
The bonds are very thin and slippage between the laminar layers do not occur. This
means that the displacements are not discontinuous across the laminas boundaries.
The strain normal to the neutral surface is ignored.
Post buckling the line which is straight and normal to the mid plane remains straight
and mid plane.
Figure 2
Layers of a laminate composite plate [2]
To derive the governing buckling equations we here consider the classical laminate theory. We
consider the equilibrium of the forces and the moments to derive the governing equations of
buckling. [2]
9
Balancing the forces the equilibrium equation can be written as (Figure 2):
0x xyN N
x y
0xy yN N
x y
………. (1)
Where Nxy; Ny; and Nx are the forces which act inside the ply in perpendicular direction and
tangential direction.
Balancing the moments the equilibrium equation can be written as (Figure 2):
2 2 2 2 2 2
2 2 2 22 2 0
x xy yx y xy
M M M w w wN N N
x x y y x y x y
………………………(2)
where, Nx ;Ny; Nxy are the forces acting on the edge of the plate.
Figure 3
Forces acting on the plate [2]
Figure 4 : Moments acting on the plate [2]
10
The resultant forces Nx; Ny and Nxy and moments Mx; My and Mxy can be obtained bt
integrating the stress acting on each layer through the thickness of the plate. Knowing the
stress in terms of the displacement, the stress resultant can be obtained as follows in terms
of Mx ; My ; and Mxy., Nx; Ny; Nxy;
The stress resultants are defined as:
/2
/2
t
x X
t
N dz
/2
/2
t
y y
t
N dz
/2
/2
t
xy xy
t
N dz
/2
/2
t
x x
t
M zdz
/2
/2
t
y y
t
M zdz
/2
/2
t
xy xy
t
M zdz
…………………… (3)
Where x , y and xy are normal and shear stress.
Strictly speaking the above forces are the forces which are shown in Figure 3 act per unit length
of the laminate. Similarly, the above moments as shown in Figure 4 act per unit length of the
laminate. Thus, the forces and moments for an N-layer laminate can be defined as:
/2
1/2 1
x x xh ZrN
y y y
rh Zrxy xy xy
r r
N
N dz dz
N
…………………………….. (4)
/2
1/2 1
x x xh ZrN
y y y
rh Zrxy xy xy
r r
M
M zdz zdz
M
…………………………….(5)
Zr and Zr-1 can be defined as in the figure below:
Figure 5: Laminated composite plate with detail layer number [2]
11
We must note that z0=-t/2. Substituting for x , y and xy in in equations (2) and (3) and
integrating over the thickness of each layer and adding the results so obtained for N layers, we
can write the stress resultants as:
011 12 16 11 12 16
012 22 26 12 22 26
016 26 66 16 26 66
xx x
y y y
xy xyxy
N A A A B B B k
N A A A B B B k
N A A A B B B k
011 12 16 11 12 16
012 22 26 12 22 26
016 26 66 16 26 66
xx x
y y y
xy xyxy
M B B B D D D k
M B B B D D D k
M B B B D D D k
………………………. (6 and 7)
Where:
Aij = 1
1
( ) ( )N
ij r r r
r
Q Z Z
,
Bij = 2 2
1
1
1 / 2 ( ) ( )N
ij r r r
r
Q Z Z
,
Dij = 3 3
1
1
1 / 3 ( ) ( )N
ij r r r
r
Q Z Z
…………………………….. (8)
Here, Aij denotes the extensional stiffness, Bij denotes the coupling stiffness, and Dij denotes
the flexural stiffness. For antisymmetric laminates stress resultants are simplified in the
following sections:
In the case of angle-ply laminates where the fibre orientation alternates from lamina to
lamina as [±θ], the force and moment resultants are
011 12 11 12 16
012 22 12 22 26
066 16 26 66
0
0
0 0
xx x
y y y
xy xyxy
N A A B B B k
N A A B B B k
N A B B B k
………………………. (9)
011 12 16 11 12 16
012 22 26 12 22 26
016 26 66 16 26 66
xx x
y y y
xy xyxy
M B B B D D D k
M B B B D D D k
M B B B D D D k
…………………….. (10)
12
Such a laminate is called an anti-symmetric angle-ply laminate. If each layer in a lamina has
the same thickness then it is called a regular anti-symmetric angle-plylaminate. For such a
laminate, equations (6) and (7) reduce to:
011 12 16
012 22 26
066 16 26
0 0 0
0 0 0
0 0 0
xx x
y y y
xy xyxy
N A A B k
N A A B k
N A B B k
…………….. (11)
016 11 12
026 12 22
016 26 66
0 0 0
0 0 0
0 0 0
xx x
y y y
xy xyxy
M B D D k
M B D D k
M B B D k
…………….. (12)
Let the laminae are oriented relatively at 0o and 90o. A laminate of this type is termed as a
cross-ply laminate. Such a laminate can, again, be either symmetric cross-ply or antisymmetric
cross-ply.
Substituting for Nxy, Ny, Nx, Mx, My and Mxy from equations 9 and 10 after substituting for 0
x
, 0
y and 0
xy , xk , yk and
xyk in equations 1 and 2 we get the governing equations as follows
:
2 0 2 0 2 0 2 0 2 0 2 0 3 3
11 12 66 16 26 66 11 162 2 2 2 3 2
3 3
12 66 262 3
( ) ( 2 ) 3
( 2 ) 0
u v u u v u w wA A A A A A B B
x x y x x y y y x x y
w wB B B
x y y
2 0 2 0 2 0 2 0 2 0 2 0 3 322
16 12 66 26 66 26 16 12 662 2 2 2 3 2
3 3
26 222 3
( ) 2 ( 2 )
3 0
u u u v v v w wA A A A A A A B B B
x x y y x x y y x x y
w wB B
x y y
4 4 4 4 4 3 0 3 0 3 0
16 12 16 26 22 11 16 12 664 3 2 2 3 4 3 2 2
3 0 3 0 3 0 3 0 2 2 2
26 16 12 66 223 3 2 3 2 2
11 4 (2 4 ) 4 3 ( 2 )
( 2 ) 2x y xy
w w w w w u u uD D D D D D B B B B
x x y x y x y y x x y x y
u v v v w w wB B B B B N N N
y x x y y x y x y
All the three equations need to be solved for a general laminate as they are coupled.
13
CHAPTER 3
EXPERIMENTAL STUDY
14
NEED FOR EXPERIMENTS
Many numerical and mathematical models exist which can be used to describe the behaviour
of a laminate under the action of different forces. When it comes to buckling we can develop a
mathematical model which can be used to model the phenomenon of buckling. But numerical
methods become complicated as the number of assumptions decrease and the number of
variables increase. Also once the model is formed it takes a lot of time to solve the partial
differential equations and then arrive at the final result. This process becomes very
cumbersome and time consuming. In view of the above mentioned laminations experimental
methods are followed. The experimental processes need less time and less computational work
is involved in that. Also the result obtained in experiments is very close to that which is
obtained theoretically.
PRESENT EXPERIMENTAL SETUP
Earlier experiments have been conducted to determine the critical buckling load of the
laminated composite plates. But most of these experiments have been conducted on INSTRON
test machines. The INSTRON test machines cost very much and also they are not flexible as
once they have been installed they cannot be moved from place to place. So in this work an
indigenous buckling setup has been devised with minimum cost so that the buckling tests can
be performed at much low costs. Also the setup is flexible and can be assembled at any place
where the test is to be carried out. The setup can also be extended to do tension tests with
suitable modifications.
PREPARATION OF THE LAMINATED COMPOSITE PLATES
Composites are used in almost all disciplines of engineering. As such there are many processes
to prepare composites. Research is also going on in industries to prepare composites much
faster and the most economical way. Most of these methods have their own set of advantages
and disadvantages. The two most popular methods which are there for the preparation of
composites are hand layup technique and the spray up technique. Fabricating a composite part
is generally concerned with placing and retaining fibres in the direction and form that is
required to provide specified characteristics while the part performs its design function.
The methods of production will depend on factors such as cost, shape of components, number
of components and required performance.
15
The manufacturing process can be classified into two broad categories:
Hand methods
Mould methods
Hand methods can be further classified into hand layup and spray up techniques. Moulding
methods include Matched-die moulding and forming methods by employing gas pressure other
processes include filament winding and pultrusion process.
HAND LAYUP TECHNIQUE
Hand lay-up refers to the manual method of laying or applying the reinforcement material into
the mold. In the hand lay-up process, the reinforcing material (usually fiberglass mat) is placed
in the mold and then saturated with polyester resin using a brush or a two-component spray
system.
Advantages of hand layup techniques:
•Widely used for many years.
•Simple principles to teach.
•Low cost tooling, if room-temperature cure resins are used.
•Wide choice of suppliers and material types.
•Higher fibre contents and longer fibres than with spray lay-up.
Figure 6
Hand lay-up technique
16
PROCEDURE FOR THE PREPARATION OF LAMINATED COMPOSITE PLATES
The composites have two components. The first is the matrix which acts as the skeleton of the
composite and the second is the hardener which acts as the binder for the matrix. The
reinforcement that was used for the project was woven glass fibres. Glass fibres are materials
which consist of numerous extremely fine fibres of glass. It is used as a reinforcing agent for
many polymer products; to form a very strong and light fibre (FRP) composite
material called glass-reinforced plastic (GRP), popularly known as "fiberglass". The woven
glass fibre was procured from the market and was used as the reinforcement for the composite.
The hardener that was utilized was epoxy. Epoxy is obtained as the last item in the wake of
curing the saps. It is likewise utilized as a solid cement for staying things together and
disguising surfaces. When poly epoxides respond with themselves or regular hardener then we
get a thermosetting polymer, regularly with solid mechanical properties and high temperature
and substance safety.
(a) Glass fibre
(b) Epoxy Figure 7 Presents the individual component of the composite
17
HAND LAYUP PROCESS OF COMPOSITE MANUFACTURING
To manufacture the composites the following steps were followed.
1. The weight of the fibre was noted down. Then approximately 1/3rd mass of the hardener
of epoxy was prepared for further use.
2. A clean plastic sheet was taken and the mould releasing spray was sprayed on it. After
that a generous coating of the hardener mixture was coated on the sheet.A woven fibre
sheet was taken and placed on top of the coating. After this again the coating of hardener
was done. A second layer of fibre was placed and the process continued until the
required thickness was obtained. The fibre was pressed with the help of rollers.
3. Another plastic sheet was taken and the mould releasing spray was sprayed on it. The
plastic sheet was placed on top of the fibre with hardener coating.
4. The plate obtained was placed under weights for a period of 24 hours.
5. After that the plastic sheets were removed and the plates separated.
Figure 8 (a) Figure 8 (b)
Figure 8 (c) Figure 8 (d)
18
Figure 8 (e) Figure 8 (f)
FABRICATION OF BUCKLING TEST RIG
The buckling test rig was developed in the Central Workshop of NIT Rourkela. The frame was
built using rectangular shaped mild steel channels. The channels were welded to one another
and then the frame was prepared. A 10 tonne hydraulic jack was assembled into the frame to
provide the necessary hydraulic force for the compression of the plates. The setup can be
assembled an disassembled at will as all its components can be separated. Thus the setup offers
flexibility over the conventional buckling setups.
Figure 9: Lab scale hydraulic buckling test rig
19
ANSYS CODE DEVELOPMENT
ANSYS is an analysis software which makes use of FEA to study and analyse the behaviour
of structures under various boundary conditions. An ANSYS code was developed which
analysed the critical buckling loads of laminated composite plates. The material properties were
picked from a journal and the results were validated. The results obtained were fairly accurate.
20
CHAPTER 4
RESULTS AND DISCUSSIONS
21
4.1. Results and Discussion
In this section, a simulation model has been developed in ANSYS parametric design language
in ANSYS environment. The model has been compared and the convergence has been checked.
Finally, the critical buckling load parameters are obtained for laminated plates for different
mode shapes and thickness ratio.
The material properties used in the present analysis are as follows:
E22=1×103, E11=3E22 and 10E22, E33=E11
G12=G22=0.6×E12, G23=0.5×E12
11 12 13 0.25
4.2 Convergence Study
In this section the convergence behaviour of laminated plate is obtained using the material,
geometry and support conditions same as the reference [1]. It is clear that the present results
are converging well with the mesh refinement.
10x10 15x15 20x20 25x25 30x30 35x35 40x40
0
5
10
15
20
25
No
nd
ime
nsio
na
l cri
tica
l b
ucklin
g lo
ad
Mesh Size
a/h=100, E1/E2=3
22
4.3 Comparison Study
The present model is being validated by comparing the results with the reference by taking the
same geometrical and material properties as well as the support conditions as stated in
reference. The comparison study has been obtained for two different laminations and presented
in Table 1 and Table 2. It is clear that the present results are showing good agreement with the
reference and present results are showing higher side as compared to the reference. It is because
of the fact that the present model is developed in the FSDT whereas in the reference the model
is developed in the HSDT.
Table. 1 Comparison study of buckling load for cross ply [0/90/0] laminated composite
plate.
a/h E11/E22 Non-dimensional critical buckling load
(Ncr) Present
Reference [1]
10
3 5.4702 5.3933
10 8.6645 9.9406
100 3 6.8984 5.1245
10 14.1641 11.4847
Table. 2 Comparison study of buckling load for cross ply [0/90/90/0] laminated composite
plate.
a/h E11/E22 Non-dimensional critical buckling load
(Ncr) Present
Reference [1]
10
3 5.3215 5.4120
10 9.7154 10.0130
100 3 5.6521 5.7616
10 10.6945 11.4813
23
4.3.1 New Illustration
Here, in this section some new results are obtained for two different parameters (thickness ratio
and orthotropicity) of simply supported cross-ply [0/90/90] laminated plate. The responses are
presented in Table 3 and Table 4. It is observed that, the buckling load increases with thickness
ratio and orthotropicity.
Table. 3: Effect of thickness ratio (a/h) on buckling load
a/h Nondimensional Buckling load
10 3.3524
20 4.5964
50 5.0243
100 6.8746
Table. 4: Effect of thickness orthotropicity on buckling load
E1/E2 Nondimensional Buckling load
3 3.3524
10 4.1107
20 5.0457
30 5.8487
24
4.3.2Buckling mode shape
In this section first four mode shapes are for simply supported cross ply lamination and
obtained using ANSYS and presented in the Fig. 10.
Figure 10: Different buckling mode shapes of laminated composite plate
25
CHAPTER 5
CONCLUSION
26
An APDL code was developed in ANSYS and the code was run. The dimensional critical
buckling load and the non-dimensional critical buckling load were obtained. The non-
dimensional critical buckling load obtained was compared with a standard literature. The
results obtained were in agreement with the standard literature.
As the lamination scheme changes the critical buckling load does not get affected much. This
is evident by the similar critical buckling loads obtained for the [0/90/0] and [0/90/90/0]
composites.
The critical buckling load is strongly dependent on the elasticity along the X axis as is evident
from the results obtained. The critical buckling load nearly doubles when the ratio E1/E2
changes from 3 to 10. This is because the plate is subjected to uniaxial loading along the X
direction.
The locally manufacture buckling setup was prepared with very little cost and in a short span
of time. This ensured that experiments can be conducted with the help of minimum cost and
with a fair degree of accuracy.
27
CHAPTER 6
REFERENCES
28
[1] S. Singh, J. Singh, K. K. Shukla, Buckling of laminated composite plates subjected to
mechanical and thermal loads using meshless collocations, Journal of Mechanical
Science and Technology 27 (2) (2013)-327-336
[2] Arum Kumar R, Buckling Analysis of woven glass epoxy laminated composite Plate,
M.Tech thesis submitted by, 2009, Department of civil engineering, NIT Rourkela.
[3] Schlack, Alois,L, Jr. “ Elastic stability of pierced square plates” , Experimental
Mechanics, DRYDEN Flight Research Center, PP.167-175, 1964
[4] Martin, James “Buckling and post buckling of laminated composite square plates with
reinforced central holes”. Ph.D. Diss.,Case Western Reserve Univ., 1972.
[5] Marshall,I,H,. Little,W,. El Tayeby,M, M,.Williams,J, “ Buckling of perforated
composite plates – an approximate solution”. Proceedings of the Second International
Conference on Fiber Reinforced Composites , Mech. Eng. Publ.,pp,29-33, 1986.
[6] Nemethm , Michael, P,. Stein, Manuel. Johnson, Eric, R, “An approximate buckling
analysis for rectangular orthotropic plates with centerally located cutouts”. NASA TP-
2528, 1986.
[7] Lee, Y,J,. Lin, H,J,. Lin, C,C,. “ A study on the buckling behavior of orthotropic square
plate with a central circular hole”, composite structural. Vol. 13, no.3, pp.173-
188,1989.
[8] Lin, Chien- Chang; and Kuo, Ching- Suong.” Buckling of Laminated Plates with
Holes”. J. Composit. Mater, vol. 23, June 1989, pp.536-553s.
[9] Ko, William, L, “ Mechanical- and thermal – buckling behavior of rectangular plates
with different central cutouts”, NASA-TM- 1998-206542,1998.
[10] Rouse, Marshall “ Effect of cutouts or low – speed impact damage on the postbuckling
behavior of composite plates loaded in shear”. Proceedings of the 31st AIAA, ASME,
ASCE, ASC, Structures, Structural Dynanics and Materials Conference, pp.877-
891,1990.
[11] Yasui, Yoshiaki “ The buckling of rectangular composite plates with cutout under
uniaxial and biaxial compression”. Proceedings the 18th International Conference on
Composite Materials,pp.4-B-1– 4-B-8,1991.
[12] Jameel, H, Therib “ An investigation of elastic buckling for perforated plates in
aircraft structures” M.Sc. thesis , Al-Rasheed College , of Engineering and Science,
University of Technology, 2004
29